Nitrogen containing carbon nanotubes as supports for
Pt – Alternate anodes for fuel cell applications
T. Maiyalagan, B. Viswanathan *, U.V. Varadaraju
Department of Chemistry, Indian Institute of Technology Madras, Chennai 600 036, India
Received 7 June 2005; accepted 7 July 2005
Available online 8 August 2005
Aligned nitrogen containing carbon nanotubes have been synthesized using Anodisc alumina membrane as template. Highly dis-
persed platinum nanoparticles have been supported on the nitrogen containing carbon nanotubes. Nitrogen containing carbon
nanotubes as platinum catalyst supports were characterized by electron microscopic technique and electrochemical analysis. The
EDX patterns show the presence of Pt and the micrograph of TEM shows that the Pt particles are uniformly distributed on the
surface of the nitrogen containing carbon nanotube with an average particle size of 3 nm. Cyclic voltammetry studies revealed a
higher catalytic activity of the nitrogen containing carbon nanotube supported Pt catalysts.
Ó 2005 Elsevier B.V. All rights reserved.
Keywords: Nitrogen containing carbon nanotubes; Template synthesis; Alumina template; Catalyst support; Methanol oxidation
Since the last decade, fuel cells have been receiving an
increased attention due to the depletion of fossil fuels
and rising environmental pollution. Fuel cells have been
demonstrated as interesting and very promising alterna-
tives to solve the problem of clean electric power gener-
ation with high eﬃciency. Among the diﬀerent types of
fuel cells, direct methanol fuel cells (DMFCs) are excel-
lent power sources for portable applications owing to its
high energy density, ease of handling liquid fuel, low
operating temperatures (60–100 °C) and quick start up
[1,2]. Furthermore, methanol fuel cell seems to be highly
promising for large-scale commercialization in contrast
to hydrogen-fed cells, especially in transportation .
The limitation of methanol fuel cell system is due to
low catalytic activity of the electrodes, especially the an-
odes and at present, there is no practical alternative to
Pt based catalysts. High noble metal loadings on the
electrode [4,5] and the use of perﬂuorosulfonic acid
membranes signiﬁcantly contribute to the cost of the de-
vices. An eﬃcient way to decrease the loadings of pre-
cious platinum metal catalysts and higher utilization of
Pt particles is by better dispersion of the desired metal
on the suitable support . In general, small particle size
and high dispersion of platinum on the support will re-
sult in high electrocatalytic activity. Carbon materials
possess suitable properties for the design of electrodes
in electrochemical devices. Carbon is an ideal material
for supporting nano-sized metallic particles in the elec-
trode for fuel cell applications. No other material except
carbon material has the essential properties of electronic
conductivity, corrosion resistance, surface properties,
and the low cost required for the commercialization of
fuel cells. In general, the conventional supports namely
carbon black is used for the dispersion of Pt particles .
The appearance of novel carbon support materials,
such as graphite nanoﬁbers (GNFs) [8,9], carbon nano-
tubes (CNTs) [10–17], carbon nanohorns , and car-
bon nanocoils [19–22], provides new opportunities of
1388-2481/$ - see front matter Ó 2005 Elsevier B.V. All rights reserved.
Corresponding author. Tel.: +91 044 22574200; fax: +91 44
E-mail address: email@example.com (B. Viswanathan).
Electrochemistry Communications 7 (2005) 905–912
carbon supports for fuel cell applications. Bessel et al. 
and Steigerwalt et al.  used GNFs as supports for Pt
and Pt–Ru alloy electrocatalysts and observed better
activity for methanol oxidation. The high electronic
conductivity of GNFs and the speciﬁc crystallographic
orientation of the metal particles resulting from well-
ordered GNF support were believed to be the important
factors for the observed enhanced electrocatalytic activ-
ity. The morphology and the nature of the functional
groups of the support inﬂuence the activity of fuel cell
electrocatalyts [23–26]. Carbon with sulphur or nitrogen
based functionality , can inﬂuence the activity of the
The present report focuses on the eﬀorts undertaken
to develop unconventional supports based platinum
catalysts for methanol oxidation. Nitrogen containing
carbon nanotubes were used to disperse the platinum
particles eﬀectively without sintering and to increase
the catalytic activity for methanol oxidation. The tubu-
lar morphology and the nitrogen functionality of the
support have inﬂuence on the dispersion as well as
the stability of the electrode. In this communication
the preparation of highly dispersed platinum supported
on nitrogen containing carbon nanotubes, the evalua-
tion of the activity for the methanol oxidation of these
electrodes and comparison with the activity of conven-
tional electrodes are reported.
All the chemicals used were of analytical grade. Poly-
vinyl pyrrolidone (Sisco Research Laboratories, India),
dichloromethane and concentrated HF (both from
Merck) were used. Hexachloroplatinic acid was ob-
tained from Aldrich. 20 wt% Pt/Vulcan carbons were
procured from E-TEK. Methanol and sulphuric acid
were obtained from Fischer chemicals. The alumina
template membranes (Anodisc 47) with 200 nm diameter
pores were obtained from Whatman Corp. Naﬁon
5 wt% solution was obtained from Dupont and was used
2.2. Synthesis of nitrogen containing carbon nanotubes
Pyrolysis of nitrogen containing polymers is a facile
method for the preparation of carbon nanotube materi-
als containing nitrogen substitution in the carbon frame-
work. Nitrogen containing carbon nanotubes were
synthesized by impregnating polyvinylpyrrolidone
(PVP) inside the alumina membrane template and subse-
quent carbonization of the polymer . Polyvinylpyr-
rolidone (PVP – 5 g) was dissolved in dichloromethane
(20 ml) and impregnated directly in the pores of the
alumina template by wetting method . After
complete solvent evaporation, the membrane was placed
in a quartz tube (30 cm length, 3.0 cm diameter), kept in
a tubular furnace and carbonized at 1173 K under Ar
gas ﬂow. After 3 h of carbonization, the quartz tube
was cooled to room temperature. The resulting template
with carbon–nitrogen composite was immersed in 48%
HF at room temperature for 24 h to remove the alumina
template and the nitrogen containing CNTs were
obtained as an insoluble fraction. The nanotubes were
then washed with distilled water to remove the residual
HF and dried at 393 K.
2.3. Loading of Pt catalyst inside nanotube
Platinum nanoclusters were loaded inside the N-CNT
as follows; the C/alumina composite obtained (before
the dissolution of template membrane) was immersed
in 73 mM H2PtCl6 (aq) for 12 h. After immersion, the
membrane was dried in air and the ions were reduced
to the corresponding metal(s) by a 3 h exposure to ﬂow-
ing H2 gas at 823 K. The underlying alumina was then
dissolved by immersing the composite in 48% HF for
24 h. This procedure resulted in the formation of Pt
nanocluster loaded N-CNT and the complete removal
of ﬂuorine and aluminum was conﬁrmed by EDX
2.4. Preparation of working electrode
Glassy carbon (GC) (Bas electrode, 0.07 cm2
polished to a mirror ﬁnish with 0.05 m alumina suspen-
sions before each experiment and served as an underly-
ing substrate of the working electrode. In order to
prepare the composite electrode, the nanotubes were
dispersed ultrasonically in water at a concentration of
1 mg mlÀ1
and 20 ll aliquot was transferred on to a
polished glassy carbon substrate. After the evaporation
of water, the resulting thin catalyst ﬁlm was covered
with 5 wt% Naﬁon solution. Then the electrode was
dried at 353 K and used as the working electrode.
2.5. Characterization methods
The chemical composition of the nanotubes was
determined by elemental analysis using Hereaus CHN
analyzer after the removal of alumina template. The
scanning electron micrographs were obtained using
JEOL JSM-840 model, working at 15 keV. The nano-
tubes were sonicated in acetone for 20 min and then
were dropped on the cleaned Si substrates. The AFM
imaging was performed in air using the Nanoscope IIIA
atomic force microscope (Digital Instruments, St. Bar-
bara, CA) operated in contact mode. For transmission
electron microscopic studies, the nanotubes dispersed
in ethanol were placed on the copper grid and the
906 T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912
images were obtained using Phillips 420 model, operat-
ing at 120 keV.
2.6. Electrochemical measurements
All electrochemical studies were carried out using a
BAS 100 electrochemical analyzer. A conventional
three-electrode cell consisting of the GC (0.07 cm2
working electrode, Pt plate (5 cm2
) as counter electrode
and Ag/AgCl reference electrode were used for the cyclic
voltammetry (CV) studies. The CV experiments were
performed using 1 M H2SO4 solution in the absence
and presence of 1 M CH3OH at a scan rate of
50 mV sÀ1
. All the solutions were prepared by using ul-
tra pure water (Millipore, 18 MX). The electrolytes were
degassed with nitrogen gas before the electrochemical
3. Results and discussion
Elemental analysis was conducted to examine
whether nitrogen has really entered the carbon nanotube
framework. It has been found that the samples prepared
contained about 87.2% carbon and 6.6% nitrogen (w/w).
The SEM images of the nitrogen containing carbon
nanotubes support are shown in Fig. 1(a)–(c). Top view
of the vertically aligned nitrogen containing carbon
nanotubes is shown in Fig. 1(a). Fig. 1(b) shows lateral
view of the nitrogen containing carbon nanotubes with
low magniﬁcation and Fig. 1(c) shows lateral view of
the nitrogen containing carbon nanotubes with high
magniﬁcation. The hollow structure and well alignment
of the nitrogen containing carbon nanotubes have been
identiﬁed by SEM.
AFM images of the nitrogen containing carbon nano-
tubes deposited on a silicon substrate are shown in
Fig. 2. The AFM tip was carefully scanned across the
tube surface in a direction perpendicular to the tube
axis. From the AFM images, it is inferred that a part
of the long nanotube is appearing to be cylindrical in
shape and is found to be terminated by a symmetric
hemispherical cap. Because of the ﬁnite size of the
AFM tip, convolution between the blunt AFM tip and
the tube body will be giving rise to an apparently greater
lateral dimension than the actual diameter of the tube
The TEM images are shown in Fig. 3(a)–(c). The
open end of the tubes observed by TEM shows that
the nanotubes are hollow and the outer diameter of
the nanotube closely match with the pore diameter of
template used, with a diameter of 200 nm and a length
of approx. 40–50 lm. It is evident from the micrographs
that there is no amorphous material present in the nano-
tube. Fig. 3(c) shows the TEM image of Pt nanoparticles
ﬁlled carbon nanotubes. TEM pictures reveal that the Pt
Fig. 1. SEM images of the nitrogen containing carbon nanotubes: (a) the top view of the nanotubes; (b) side view of the vertically aligned nanotubes
and (c) high magniﬁcation lateral view of the nanotubes.
T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912 907
Fig. 2. AFM image of the nitrogen containing carbon nanotubes.
Fig. 3. TEM images of the nitrogen containing carbon nanotubes: (a) at lower magniﬁcation; (b) at higher magniﬁcation image of the individual
nanotube (an arrow indicating the open end of the tube) and (c) Pt ﬁlled nitrogen containing carbon nanotubes.
908 T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912
particles have been homogeneously dispersed on the
nanotubes and particle sizes were found to be around
3 nm. The optimal Pt particle size for reactions in the
H2/O2 fuel cell is 3 nm . The importance of the Pt
particle size on the activity for methanol oxidation is
due to the structure sensitive nature of the reaction
and the fact that particles with diﬀerent sizes will
have diﬀerent dominant crystal planes and hence the dif-
ferent intercrystallite distances, which might inﬂuence
methanol adsorption. The commercial Pt/C has a very
high speciﬁc surface area but contributed mostly by
micropores less than 1 nm and are therefore more diﬃ-
cult to be fully accessible. It has been reported that the
mean value of particle size for 20% Pt/Vulcan
(E-TEK) catalyst was 2.6 nm . The EDX pattern of
the as synthesized catalyst shows the presence of Pt
particles in the carbon nanotubes and also the complete
removal of ﬂuorine and aluminum has also been
conﬁrmed in Fig. 4. It has been reported that the
electronic and physical structures of a Pt particle
deposited on carbon diﬀer from those of the bulk Pt.
The electronic change in Pt/C is considered as a result
of functional groups of the carbon support that might
inﬂuence the electronic structure of Pt particulate
[32–36]. The nitrogen functional group on the carbon
nanotubes surface intensiﬁes the electron withdrawing
eﬀect against Pt and the decreased electron density of
platinum facilitate oxidation of methanol.
Fig. 5(a)–(c) shows the cyclic voltammogram of
methanol oxidation. Fig. 5(c) shows the cyclic voltam-
mogram of Pt/N-CNT electrode in 1 M H2SO4/1 M
CH3OH run at a scan rate of 50 mV sÀ1
. The electrocat-
alytic activity of methanol oxidation at the Pt/N-CNT
electrodes was evaluated and compared with that of
the conventional electrodes. During the anodic scan,
the current increases quickly due to dehydrogenation
of methanol followed by the oxidation of absorbed
methanol residues and reaches a maximum in the poten-
tial range between 0.8 and 1.0 V vs. Ag/AgCl. In the
cathodic scan, the re-oxidation of methanol is clearly
observed due to the reduction of oxide of platinum.
Electrocatalytic activity of methanol oxidation has been
found to be strongly inﬂuenced by the metal dispersion.
Pure Pt electrode shows an activity of 0.167 mA cmÀ2
The Pt/N-CNT shows a higher activity of 13.3 mA cmÀ2
where as conventional 20% Pt/Vulcan (E-TEK)
electrode shows less activity of 1.3 mA cmÀ2
to nitrogen containing carbon nanotube supported
electrode. The nitrogen containing carbon nanotube
supported electrodes shows a ten fold increase in the
catalytic activity compared to the E-TEK electrode.
The Pt/N-CNT electrode showed higher electrocatalytic
activity for methanol oxidation than commercial
Pt/Vulcan (E-TEK) electrode. The anodic current
density of Pt/N-CNT electrode is found to be higher
than that of Pt/Vulcan (E-TEK) electrode, which indi-
cates that the catalyst prepared with nitrogen containing
carbon nanotubes as the support has excellent catalytic
activity on methanol electrooxidation.
The onset potential and the forward-scan peak current
density for the diﬀerent electrodes are given in Table 1.
The onset potential of methanol oxidation at nitrogen
containing carbon nanotube supported catalysts occurs
at 0.22 V, which is relatively more negative to that of
the other catalysts. This may be attributed to the high dis-
persion of platinum catalysts and the nitrogen functional
groups on its surface. The higher electrocatalytic activity
of the nitrogen containing carbon nanotube supported
electrode is due to higher dispersion and a good interac-
tion between the support and the Pt particles The Vulcan
Fig. 4. EDX pattern of Pt/N-CNT electrode.
T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912 909
carbon support has randomly distributed pores of vary-
ing sizes which may make fuel and product diﬀusion
diﬃcult whereas the tubular three-dimensional morphol-
ogy of the nitrogen containing carbon nanotubes makes
the fuel diﬀusion easier. The Vulcan carbon contains high
levels of sulfur (ca. 5000 ppm or greater), which could
potentially poison the fuel-cell electrocatalysts .
Nitrogen containing carbon nanotubes used in this study
contains heterocyclic nitrogen so that it preferentially at-
taches the Pt particles. The selective attachment of Au
nanoparticles on nitrogen doped carbon nanotubes has
also been reported . All these results indicate that
the nitrogen functionality on CNT inﬂuences the
catalytic activity of the catalyst. The enhanced electrocat-
alytic eﬀect of the nitrogen containing carbon nanotube
supported electrodes could also be partly due to the
following factors which require further investigation:
(1) higher dispersion on the nitrogen containing carbon
nanotube support increases the availability of an
enhanced electrochemically active surface area, (2)
appearance of the speciﬁc active sites at the metal–
support boundary and, (3) strong metal–support
Long-term stability is important for practical applica-
tions. Fig. 6 shows the current density–time plots of var-
ious electrodes in 1 M H2SO4 and 1 M CH3OH at 0.6 V.
The performance of Pt electrodes was found to be poor
compared to the E-TEK and Pt/N-CNT electrode. The
nitrogen containing carbon nanotube electrodes are the
most stable for direct methanol oxidation. The increas-
ing order of stability of various electrodes is; Pt < Pt/
Vulcan (E-TEK) < Pt/N-CNT. We are currently investi-
gating whether nitrogen has a catalytic role that contrib-
Fig. 5. Cyclic voltammograms of (a) pure Pt; (b) Pt/Vulcan (E-TEK) and (c) Pt/N-CNT in 1 M H2SO4/1 M CH3OH run at 50 mV sÀ1
Electrochemical parameters for methanol oxidation on the various
Electrocatalyst Methanol oxidation
onset potential (V)
Forward peak current
density (mA cmÀ2
Bulk Pt 0.4 0.167
20% Pt/C (E-TEK) 0.45 1.3
Pt/N-CNT 0.22 13.3
910 T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912
utes to the observed enhancement in the methanol oxi-
dation. Recent experiments conducted in our laboratory
on Pt supported N-doped and undoped CNTs reveal the
importance of nitrogen functionalities on methanol oxi-
dation activity .
In summary, it is reported platinum catalysts are
highly dispersed on the surface of well-aligned
nitrogen containing carbon nanotube. The tubular
morphology and the nitrogen functionality favour
dispersion of the Pt particles. The electrocatalytic
properties of Pt particles supported on the three-
dimensional nitrogen containing carbon nanotube
electrode shows higher catalytic activity for methanol
oxidation than the commercial E-TEK electrode,
which implies that the well-aligned nitrogen containing
carbon nanotube arrays have good potential
application as a catalyst support in direct methanol
We thank the Council of Scientiﬁc and Industrial Re-
search (CSIR), India, for a senior research fellowship to
one of the authors T. Maiyalagan.
 M.P. Hogarth, G.A. Hards, Platinum Met. Rev. 40 (1996) 150.
 T.R. Ralph, Platinum Met. Rev. 41 (1997) 102.
 B.D. McNicol, D.A.J. Rand, K.R. Williams, J. Power Sources 83
 A. Hamnett, Catal. Today 38 (1997) 445.
 S. Wasmus, A. Kuver, J. Electroanal. Chem. 461 (1999) 14.
 T. Matsumoto, T. Komatsu, K. Arai, T. Yamazaki, M. Kijima,
H. Shimizu, Y. Takasawa, J. Nakamura, Chem. Commun. 7
 K. Kinoshita, Carbon: Electrochemical and Physicochemical
Properties, John Wiley, New York, 1988.
 C.A. Bessel, K. Laubernds, N.M. Rodriguez, R.T.K. Baker, J.
Phys. Chem. B 105 (6) (2001) 1115.
 E.S. Steigerwalt, G.A. Deluga, D.E. Cliﬀel, C.M. Lukehart, J.
Phys. Chem. B 105 (34) (2001) 8097.
 B. Rajesh, V. Karthik, S. Karthikeyan, K.R. Thampi, J.M.
Bonard, B. Viswanathan, Fuel 81 (2002) 2177.
 Z.L. Liu, X.H. Lin, J.Y. Lee, W.D. Zhang, M. Han, L.M. Gan,
Langmuir 18 (2002) 4054.
 W.Z. Li, C.H. Liang, W.J. Zhou, J.S. Qiu, Z.H. Zhou, G.Q. Sun,
J. Phys. Chem. B 107 (2003) 6292.
 T. Matsumoto, T. Komatsu, H. Nakano, K. Arai, Y. Nagashima,
E. Yoo, T. Yamazaki, M. Kijima, H. Shimizu, Y. Takasawa, J.
Nakamura, Catal. Today 90 (2004) 277.
 C. Kim, Y.J. Kim, Y.A. Kim, T. Yanagisawa, K.C. Park, M.
Endo, M.S. Dresselhaus, J. Appl. Phys. 96 (2004) 5903.
 Yangchuan Xing, J. Phys. Chem. B 108 (50) (2004) 19255.
 C. Wang, M. Waje, X. Wang, J.M. Tang, C.R. Haddon, Y. Yan,
Nano Lett. 4 (2) (2004) 345.
 M. Carmo, V.A. Paganin, J.M. Rosolen, E.R. Gonzalez, J. Power
Sources 142 (2005) 169.
 T. Yoshitake, Y. Shimakawa, S. Kuroshima, H. Kimura, T.
Ichihashi, Y. Kubo, D. Kasuya, K. Takahashi, F. Kokai, M.
Yudasaka, S. Iijima, Physica B 323 (2002) 124.
 T. Hyeon, S. Han, Y.E. Sung, K.W. Park, Y.W. Kim, Angew.
Chem. Int. Ed. 42 (2003) 4352.
 K.W. Park, Y.E. Sung, S. Han, Y. Yun, T. Hyeon, J. Phys. Chem.
B 108 (2004) 939.
 G.S. Chai, S.B. Yoon, J.S. Yu, J.H. Choi, Y.E. Sung, J. Phys.
Chem. B 108 (2004) 7074.
 S.H. Joo, S.J. Choi, I. Oh, J. Kwak, Z. Liu, O. Terasaki, R. Ryoo,
Nature 412 (2001) 169.
 M. Uchida, Y. Aoyama, M. Tanabe, N. Yanagihara, N. Eda, A.
Ohta, J. Electrochem. Soc. 142 (1995) 2572.
 S.C. Roy, P.A. Christensen, A. Hamnett, K.M. Thomas, V.
Trapp, J. Electrochem. Soc. 143 (1996) 3073.
 A.K. Shukla, M.K. Ravikumar, A. Roy, S.R. Barman,
D.D. Sarma, A.S. Arico, J. Electrochem. Soc. 141 (1994)
 S. Ye, A.K. Vijh, L.H. Dao, J. Electrochem. Soc. 144 (1997)
 T. Maiyalagan, B. Viswanathan, Mater. Chem. Phys. 93 (2005)
 M. Steinhart, J.H. Wendorﬀ, A. Greiner, R.B. Wehrspohn,
K. Nielsch, J. Schilling, J. Choi, U. Goesele, Science 296 (2002)
 S.C. Tsang, P. de Oliveira, J.J. Davis, M.L.H. Green, H.A.O. Hill,
Chem. Phys. Lett. 249 (1996) 413.
 K. Kinoshita, J. Electrochem. Soc. 137 (1990) 845.
 E. Antolini, L. Giorgi, F. Cardellini, E. Passalacqua, J. Solid State
Electrochem. 5 (2001) 131.
 S.C. Hall, V. Subramanian, G. Teeter, B. Rambabu, Solid State
Ionics 175 (2004) 809.
 P.L. Antonucci, V. Alderucci, N. Giordano, D.L. Cocke, H. Kim,
J. Appl. Electrochem. 24 (1994) 58.
 M.C. Roman-Martinez, D. Cazorla-Amoros, A. Linares-
Solano, C. Salinas-Martinez de Lecea, Curr. Top. Catal. 1
 M.C. Roman-Martinez, D. Cazorla-Amoros, A. Linares-Solano,
C. Salinas-Martinez de Lecea, H. Yamashita, M. Anpo, Carbon
33 (1) (1995) 3.
 C.G. Vayenas, S. Bebelis, C. Pliangos, S. Brosda, D. Tsiplakides,
Electrochemical Activation of Catalysis, Promotion, Electrochemical
Fig. 6. Current density vs. time curves at (a) Pt/N-CNT; (b) Pt/Vulcan
(E-TEK) and (c) Pt measured in 1 M H2SO4 + 1 M CH3OH. The
potential was stepped from the rest potential to 0.6 V vs. Ag/AgCl.
T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912 911
Promotion, and Metal–support Interactions, Kluwer, New York,
 K.E. Swider, D.R. Rolison, J. Electrochem. Soc. 143 (3) (1996)
 K. Jiang, A. Eitan, L.S. Schadler, P.M. Ajayan, R.W. Siegel, N.
Grobert, M. Mayne, M. Reyes-Reyes, H. Terrones, M. Terrones,
Nano Lett. 3 (3) (2003) 275.
 T. Maiyalagan, B. Viswanathan, U. Varadaraju, in preparation.
912 T. Maiyalagan et al. / Electrochemistry Communications 7 (2005) 905–912